Upload
others
View
4
Download
0
Embed Size (px)
Strength from Stiffness (Ultimate Properties Must Be
Considered Relative To Stiffness) David A. Anderson, PhD, PE
Professor Emeritus, Penn State
Geoffrey M. Rowe, PhD, PE Abatech
FHWA Asphalt Binder ETG
Oklahoma City, OK September 15-16, 2015
Ultimate Properties – What Are They?
Property that can be used to characterize or rank a material at the time of rupture Attempt to rank material according to their propensity to
rupture when loaded Loading may be caused by applied stress, strain Mechanically or thermally induced
Wide range from “fundamental” to empirical Used in research as well as “index” properties for
specification use Review of literature shows all obey time-temperature
superposition
Slide -2-
Ultimate Property Tests – Some Examples
Strength Not fundamental property Value depends upon specimen size and configuration Easy to measure
Fracture Properties Properties independent of specimen size and configuration Difficult to measure – require viscoelastic characterization
Energy to Failure – Cohesive energy to fracture Not fundamental property Value depends upon size and configuration Easy to measure
Slide -3-
Theme of Today’s Presentation
Ultimate properties depend upon test temperature and rate of loading For specification purposes an ultimate property must be
determined at the use temperature Specifying and ultimate property a single temperature for
all binder grades will give misleading results Ultimate properties obey time-temperature equivalency Linear viscoelastic time-temperature shift functions also
define time-temperature dependency of ultimate properties
Slide -4-
Linear visco elastic parameters – test conditions Measurements at small strain areas BBR, DSR measurements Used to generate numerical time-temperature algorithm
and material dependent parameters Note: Literature for a wide range of materials shows that both linear, non-linear, and empirical index properties obey time-temperature superposition
Stiffness - Linear visco-elastic parameters
Slide 5
Ultimate Properties – Test Parameters
What is an ultimate property? Stress/strain at break Energy Fracture property Etc.
Objective of today’s presentation ………………….. To illustrate how rheology can be used as a descriptive tool
for ultimate properties The demonstrate that an understanding of rheology is
necessary to properly interpret and use ultimate properties 3 major items to be considered
Slide 6
Issue 1: Strength versus temperature
Historical Perspective Wide variety of research where strength is normalized
with respect to temperature Huekelom (AAPT 1966) essential reading Ferry, Viscoelastic Properties of Polymers, 3rd Edition Strategic Research Program DTT Test, SHRP A-369 (1994) Polymers in non-asphalt literature, extensive literature Mixtures, FENIX test, Constr. and Bldg. Materials, (2012),
pp 372-380.
Slide -7-
Similar results for polymers
Example: Styrene-butadiene
rubber Tensile strain Data is shifted to a
reduced strain rate that captures both time and temperature
Ferry’s Book (T. Smith data)
Slide 8
Styrene-butadiene rubber
Tensile strength Data is shifted to
a reduced strain rate that captures both time and temperature
Ferry’s Book (T. Smith data)
Slide 9
Tens
ile S
tren
gth
Log10 strain rate
Heukelom (1966)
Stiffness Modulus of Bitumen, kg/cm2
10 100 1,000 10,000
10
20
30
40
50
Tens
ile S
tren
gth,
kg/
cm2 Tensile strength
of binder is a function of binder stiffness (Sb) and can be presented as master curve; Sb considers both time of loading and temperature.
This location equates to G*≈15MPa
Hukelom, AAPT, vol 35, p 358, “Observations on the rheology and
fracture of bitumens and asphalt mixtures”
Slide 10
Extended testing to mixtures with same result
Done for 8-mix types
Heukelom (1966)
Slide 11
1.0
OF M
IX
TENS
ILE S
TREN
GTH
MAXI
MUM
TENS
ILE S
TREN
GTH
0.5
0.4
0.2
0.0
0.8
SHRP A-369, Anderson et. al (1994)
Failure master curves of stress, strain and energy for conventional binders
Functional form for energy
12
Note – reduced time – not adjusted to stiffness
SHRP A-369, Anderson et. al (1994)
Also looked at SECANT modulus at failure from DTT test
Secant modulus can be considered as a “binder stiffness”
Produces single curve for all binders tested during SHRP 2A Project
13
Stiffness important to describe strength, strain and properties at break Could use other parameters that include effect of time
and temperature Stiffness is conceptually easy to understand since we
use it as a specification parameter Could use S(t), G*, E(t), etc.
Properties are both a function of loading rate and temperature! Applies to range of visco-elastic materials, bitumen,
asphalt mixes, rubber, SBS, others, etc. All practical materials going into HMA!
Summary - Item 1
Slide 14
Fatigue and fracture will exhibit a brittle to instability flow (ductile) transition!
Item 2 - Brittle to instability flow (ductile)
Slide 15
Stiffness can be used to define the transition between “ductile” and “brittle” failure Not a single stiffness value bit range Perhaps better said between brittle and brittle-ductile
behavior Failure mechanism changes as pass through transition “True” fatigue behavior with crack propagation in
traditional sense occurs below this transition Crack formation by viscous flow above transition
Definition of brittle and definition via yield stress associated presence controversial at least!
Item 2
Slide 16
Typical Stress-Strain Curves
0
2
4
6
8
0 5 10Failure strain, percent
Failu
re S
tress
, MP
a
1
AB C
DE
εf
σf
5 Test Temperatures
Slide 17
At test conditions used in DTT approximately equal to 300 MPa in BBR at 60s
Linear VE – Not nonlinear
Linear VE limit
Observations from DSR “Fatigue” Test
Evolution of failure in LAS test Observe flow above room temperature
Slide -18-
0
20
40
60
80
100
120
140
5 10 15 20 25 30Temperature (°C)
Num
ber
of c
ycle
s at
fa
ilure
, 100
0
0
10
20
30
40
50
60
Stif
fnes
s m
odul
us (M
Pa)Nf
G* (MPa)
"True" fatigue Instability flow
“Fatigue” vs. Temperature
Anderson, Marasteanu, Planche, Martin and Gauthier - Evaluation of Fatigue Criteria for Asphalt Binders – TRB 2001
Slide 19
Range in stiffness where fatigue cracking and instability flow dominate
Note that values are in same range as presented above for strength Stiffness normalizes the effect of temperature and loading
rate
Stiffness range where instability flow dominates
Binder Fatigue cracking
Instability flow
Unmodified 28 to 55 MPa 5 to 18 MPa SB crosslinked 15 to 45 MPa 5 to 10 MPa EVA modified 13 to 45 MPa 5 to 9 MPa
Slide 20
Item 3
Importance of loading speed on temperature window Temperature window depends upon speed of loading Example demonstrated with Vialit Cohesion Test
Slide -21-
22
Example of a cohesion fracture test
Fracture properties and temperature
0
100
200
300
400
500
600
700
800
-40 -20 0 20 40 60 80
Temperature (C)
DTT
- En
ergy
(J)
0
0.2
0.4
0.6
0.8
1
1.2
1.4
1.6
Vial
it - E
nerg
y (J
/cm
2)
DTT Test Vialit Test – Cohesion
Brittle
Brittle Flow/Ductile
Flow/Ductile
This shift is just related to loading time/rate! Width is related to rate!
Really a stiffness effect – needed to explain these brittle to ductile transitions.
Slide 23
Energy plots for DTT data – Energy to failure vs. Modulus
E(t) = 1MPa to 1000 MPa
Normalization of ultimate of fracture properties via linear visco-elastic modulus.
Slide 24
If using E(t) – previously observed flow/ductile to brittle range covered from about 1MPa to 1000 MPa
Note G*≈ E(t)/3 300 kPa to 300 MPa – 3.0x109 to 3x108 Pa
CA model fit works well in limited range 105 to 109 Pa This range covers stiffness range above where we would
describe fracture behavior We use the CA model to generate isochronal plot for
stiffness in this range
Range of stiffness needed
Slide 25
Rate of loading effects
Rate of loading effects range of results that will be obtained in temperature domain if properties are dependent upon stiffness as shown earlier.
Rate of any fracture test is key to understanding behavior.
Slide 26
Loading rate versus temperature range, assessed from DSR data
The loading rate in Vialet and DTT can be used to generate isochronal plot for each test
A fast rate will give a shorter temperature range since
Slide 27
Range is dependent upon assessed rate of loading of test being used
Lower Tail
Peak
Fracture properties and temperature
0
100
200
300
400
500
600
700
800
-40 -20 0 20 40 60 80
Temperature (C)
DTT
- En
ergy
(J)
0
0.2
0.4
0.6
0.8
1
1.2
1.4
1.6
Vial
it - E
nerg
y (J
/cm
2)
DTT Test Vialit Test – Cohesion
Brittle
Brittle Ductile
Ductile
This shift is just related to loading time/rate! Width is related to rate! Really a stiffness effect – needed to explain these brittle to
ductile transitions.
Slide 28
Fracture Properties from Double Notched Test in Tension
Strain: ε = δ L / L
L
Evaluation of Elastic, Plastic, and VE Fracture Mechanics Parameters
Ranking depends on methodology Ranking at equi-toughness
-30
-25
-20
-15
-10
-5
0 GSL TSL YSL PSL NSL ASL CSL RSL ESL
Low
-tem
pera
ture
spe
cific
atio
n te
mpe
ratu
res
Tcr Tk100 TJ100 TJV100
Bars left to right: 1. S and m 2. LEFM (KIC) 3. Elastoplastic (JIC) 4. Viscoelastic (JVC)
31
Use of Tg as reference temperature when analyzing fracture mechanics parameters
0,E+00
5,E+02
1,E+03
2,E+03
2,E+03
3,E+03
3,E+03
-25 -20 -15 -10 -5 0Temperature (°C)
JIC
(N/m
)
ASL CSLESL GSLNSL PSLRSL TSLYSL
0,E+00
5,E+01
1,E+02
2,E+02
2,E+02
3,E+02
3,E+02
4,E+02
4,E+02
5,E+02
5,E+02
0 2 4 6 8 10 12 14 T-Tg (°C)
J VC (N
/m)
ASL CSL ESL GSL NSL PSL RSL TSL YSL
Plotted vs T - Tg
Plotted vs. Temperature
Equivalent to using Stiffness as reference
or normalization temperature!
Item 3
Temperature window – of interest depends on the rate of loading
Slide -32-
How do we use all of this …..
Helps us to interpret data, test condition, loading configurations, etc.
Need to assess existing and new methods in rational manner
Time-temperature dependency can be determined from simplified testing – beyond scope of today’s presentation – rheology 101 for March 2016? Time-temperature algorithm is uniformly valid for rheology
and ultimate properties
Slide -33-
Item 3 – Importance of rheological behavior when evaluating ultimate properties
Rheological type Linear visco-elastic behavior relates to ultimate properties
whether they be fatigue, “cracking” strength, or whatever the property of interest may be
Can use this in analysis Can use this in testing for reasonableness
When comparing ultimate properties need to do comparison at equi-stiffness temperature Corollary: In specification test must obtain parameters
service temperature at rate consistent with service
Slide 34
Require that we determine stiffness characteristics accurately for range that effects cracking
Model stiffness master curve with BBR, DSR and CA fit with Kaelble Possible from standard data that is collected
Food for thought…… When writing a specification specify ultimate properties at
temperature and loading rate consistent with service
Items 1 to 3
Slide 35
A couple of thoughts on analysis
We have more data in data sets than we use R-value captured in all SHRP data Many ways we can estimate
Extrapolation vs. interpolation Specification parameters – property driven – will they
be the same in different climates? Rate of loading effects…. Consideration of stiffness helps us to understand tests
Slide 36
Summary
1.Stiffness – G*, E(t) is a vital element in specification-interpretation of ultimate properties 1. When conducting research carefully consider the relationship
between loading rate-temperature-stiffness 2. Ultimate binder property at single temperature-loading rate is a
poor candidate for predicting performance 2.A transition between brittle and flow-type behavior occurs at
approximately 10-30 MPa 3.The rheological type is of key importance to understand ultimate
properties/performance 4.Consequences:
1. Data collection – only use G* >1 x 105 MPa in model fits Sufficient to describing brittle to ductile fracture, etc. 1. Capture data in range of stiffness to cover transitions! 2. Linear VE time-temperature dependency of binder also relates to
cracking of mixes – thermal, fatigue, durability, etc. Dependent upon shape and position of master curve stiffness and relaxation properties
Slide 37